#------------------------------------------------------------------------------
#$Date: 2016-03-23 20:59:17 +0200 (Wed, 23 Mar 2016) $
#$Revision: 179434 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/31/4333188.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided the Crystal Eye server at
# http://wwmm.ch.cam.ac.uk/crystaleye/, created by Nick Day at the
# Peter Murray-Rust laboratory.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_4333188
loop_
_publ_author_name
'Kong, Xiang-Jian'
'Ren, Yan-Ping'
'Zheng, Pei-Qing'
'Long, Yu-Xiang'
'Long, La-Sheng'
'Huang, Rong-Bin'
'Zheng, Lan-Sun'
_publ_section_title
;
 Construction of Polyoxometalates-Based Coordination Polymers through
 Direct Incorporation between Polyoxometalates and the Voids in a 2D
 Network
;
_journal_issue                   26
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              10702
_journal_page_last               10711
_journal_paper_doi               10.1021/ic061664y
_journal_volume                  45
_journal_year                    2006
_chemical_formula_sum            'C24 H28 Cu4 N12 O42 Si W12'
_chemical_formula_weight         3645.03
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                114.618(3)
_cell_angle_beta                 99.606(3)
_cell_angle_gamma                95.554(3)
_cell_formula_units_Z            1
_cell_length_a                   11.818(2)
_cell_length_b                   12.130(2)
_cell_length_c                   12.237(3)
_cell_measurement_temperature    173(2)
_cell_volume                     1545.1(5)
_computing_cell_refinement       'SHELXTL-Plus (Sheldrick, 1990)'
_computing_data_collection       'SHELXTL-Plus (Sheldrick, 1990)'
_computing_data_reduction        'SHELXTL-Plus (Sheldrick, 1990)'
_computing_molecular_graphics    'SHELXTL V.5.0 (Sheldrick, 1997)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.918
_diffrn_measured_fraction_theta_max 0.918
_diffrn_measurement_device_type  'Bruker Smart Apex CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0553
_diffrn_reflns_av_sigmaI/netI    0.0773
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            9601
_diffrn_reflns_theta_full        25.00
_diffrn_reflns_theta_max         25.00
_diffrn_reflns_theta_min         1.88
_exptl_absorpt_coefficient_mu    23.695
_exptl_absorpt_correction_T_max  0.2530
_exptl_absorpt_correction_T_min  0.1252
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    3.917
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plate
_exptl_crystal_F_000             1610
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_refine_diff_density_max         4.652
_refine_diff_density_min         -3.850
_refine_diff_density_rms         0.561
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.060
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     430
_refine_ls_number_reflns         5002
_refine_ls_number_restraints     62
_refine_ls_restrained_S_all      1.061
_refine_ls_R_factor_all          0.0836
_refine_ls_R_factor_gt           0.0754
_refine_ls_shift/su_max          0.028
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1469P)²+0.8380P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2005
_refine_ls_wR_factor_ref         0.2083
_reflns_number_gt                4229
_reflns_number_total             5002
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic061664ysup5.cif
_cod_data_source_block           complex_5
_cod_depositor_comments
;
The following automatic conversions were performed:

'_exptl_crystal_density_meas' value 'not measured' was changed to '?'
- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 3008 2015-01-20 13:52:24Z robertas 
;
_cod_original_cell_volume        1545.2(5)
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               4333188
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
W1 W 0.17773(7) 0.79506(7) 0.03447(7) 0.0228(3) Uani 1 1 d .
W2 W 0.00537(7) 0.72720(6) -0.25698(7) 0.0246(3) Uani 1 1 d .
W3 W 0.30524(7) 1.07530(7) 0.04834(7) 0.0279(3) Uani 1 1 d .
W4 W 0.18080(7) 1.07345(8) 0.28918(7) 0.0269(3) Uani 1 1 d .
W5 W 0.12360(8) 1.01475(8) -0.23632(7) 0.0319(3) Uani 1 1 d .
W6 W 0.12825(8) 1.28675(7) 0.02605(7) 0.0286(3) Uani 1 1 d .
Si1 Si 0.0000 1.0000 0.0000 0.0180(15) Uani 1 2 d SD
O1 O 0.0972(13) 1.0680(17) -0.0289(19) 0.026(3) Uani 0.50 1 d PD
O2 O 0.009(2) 0.8672(9) -0.0437(18) 0.026(3) Uani 0.50 1 d PD
O3 O 0.011(2) 1.0606(16) 0.1377(8) 0.026(3) Uani 0.50 1 d PD
O4 O -0.1134(11) 1.0161(18) -0.0640(17) 0.026(3) Uani 0.50 1 d PD
O5 O 0.123(2) 1.178(2) -0.1401(16) 0.107(11) Uani 1 1 d .
O6 O 0.202(2) 0.9063(17) 0.2020(18) 0.092(9) Uani 1 1 d .
O7 O 0.260(2) 1.0247(19) -0.126(2) 0.074(6) Uani 1 1 d U
O8 O 0.256(3) 1.230(2) 0.0729(14) 0.112(12) Uani 1 1 d .
O9 O -0.0301(18) 1.285(2) -0.0332(15) 0.069(6) Uani 1 1 d .
O10 O 0.0988(15) 0.846(2) -0.275(3) 0.110(11) Uani 1 1 d .
O11 O 0.0372(18) 1.0086(17) 0.306(2) 0.077(7) Uani 1 1 d .
O12 O 0.123(2) 1.220(2) 0.318(2) 0.074(6) Uani 1 1 d U
O13 O 0.0998(17) 1.3320(18) 0.1814(17) 0.057(5) Uani 1 1 d U
O14 O 0.2639(18) 0.6973(18) 0.0472(17) 0.058(5) Uani 1 1 d .
O15 O 0.0042(15) 0.5956(18) -0.3788(19) 0.066(6) Uani 1 1 d .
O16 O 0.1270(16) 0.724(2) -0.1421(16) 0.079(8) Uani 1 1 d .
O17 O 0.2916(19) 1.1169(13) 0.2116(17) 0.068(7) Uani 1 1 d .
O18 O 0.2679(16) 1.1066(16) 0.4259(16) 0.054(5) Uani 1 1 d .
O19 O 0.4512(15) 1.1180(14) 0.0739(15) 0.050(5) Uani 1 1 d .
O20 O 0.289(2) 0.9113(15) 0.0218(16) 0.076(8) Uani 1 1 d .
O21 O 0.1889(13) 1.4249(13) 0.0377(15) 0.039(4) Uani 1 1 d .
O22 O 0.1797(14) 1.0159(16) -0.3505(14) 0.042(4) Uani 1 1 d .
Cu1 Cu 0.2881(3) 0.4895(5) -0.2221(4) 0.0923(17) Uani 1 1 d .
Cu2 Cu -0.2538(4) 0.1933(5) -0.4334(7) 0.135(3) Uani 1 1 d .
N1 N 0.1378(15) 0.3854(19) -0.2603(16) 0.035(4) Uani 1 1 d .
C1 C 0.047(3) 0.418(2) -0.207(2) 0.048(7) Uani 1 1 d .
H1A H 0.0650 0.4918 -0.1321 0.058 Uiso 1 1 calc R
C2 C -0.061(3) 0.3630(19) -0.245(2) 0.047(7) Uani 1 1 d .
H2A H -0.1178 0.3988 -0.2022 0.056 Uiso 1 1 calc R
C3 C -0.013(3) 0.208(2) -0.399(2) 0.055(8) Uani 1 1 d .
H3A H -0.0306 0.1264 -0.4643 0.065 Uiso 1 1 calc R
C4 C 0.110(2) 0.282(2) -0.3561(19) 0.044(6) Uani 1 1 d .
H4A H 0.1669 0.2516 -0.4017 0.053 Uiso 1 1 calc R
N2 N -0.0913(15) 0.253(2) -0.347(2) 0.043(5) Uani 1 1 d .
N3 N -0.2721(16) 0.2832(16) -0.5415(18) 0.039(4) Uani 1 1 d .
C5 C -0.332(2) 0.2319(19) -0.6682(18) 0.045(6) Uani 1 1 d DU
H5A H -0.3701 0.1481 -0.7072 0.054 Uiso 1 1 calc R
C6 C -0.3358(18) 0.2922(18) -0.7315(19) 0.029(4) Uani 1 1 d U
H6A H -0.3724 0.2503 -0.8170 0.035 Uiso 1 1 calc R
C7 C -0.235(2) 0.467(2) -0.5629(19) 0.041(6) Uani 1 1 d .
H7A H -0.1968 0.5506 -0.5266 0.049 Uiso 1 1 calc R
C8 C -0.2291(18) 0.4061(17) -0.4902(17) 0.034(5) Uani 1 1 d D
H8A H -0.1953 0.4499 -0.4042 0.040 Uiso 1 1 calc R
N4 N -0.2900(17) 0.4148(18) -0.6818(14) 0.036(4) Uani 1 1 d .
N5 N -0.390(2) 0.080(2) -0.471(2) 0.083(8) Uani 1 1 d DU
C9 C -0.425(3) -0.015(3) -0.585(2) 0.085(10) Uani 1 1 d DU
H9A H -0.3780 -0.0329 -0.6442 0.101 Uiso 1 1 calc R
C10 C -0.455(3) 0.090(3) -0.389(3) 0.089(11) Uani 1 1 d DU
H10A H -0.4229 0.1496 -0.3061 0.107 Uiso 1 1 calc R
N6 N 0.4118(18) 0.4946(18) -0.0927(16) 0.041(5) Uani 1 1 d .
C11 C 0.500(2) 0.602(2) -0.019(2) 0.041(5) Uani 1 1 d .
H11A H 0.5008 0.6732 -0.0336 0.049 Uiso 1 1 calc R
C12 C 0.5764(18) 0.6004(19) 0.0670(17) 0.030(5) Uani 1 1 d .
H12A H 0.6307 0.6749 0.1179 0.036 Uiso 1 1 calc R
O1W O -0.3429(19) 1.3683(18) -0.2573(18) 0.065(6) Uani 1 1 d .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O14 W1 O6 99.4(11) . .
O14 W1 O20 99.5(11) . .
O6 W1 O20 86.8(6) . .
O14 W1 O9 101.4(10) . 2_575
O6 W1 O9 92.6(8) . 2_575
O20 W1 O9 158.9(11) . 2_575
O14 W1 O16 99.7(10) . .
O6 W1 O16 160.7(12) . .
O20 W1 O16 86.9(8) . .
O9 W1 O16 86.8(7) 2_575 .
O14 W1 O4 160.2(8) . 2_575
O6 W1 O4 67.4(10) . 2_575
O20 W1 O4 66.2(8) . 2_575
O9 W1 O4 94.0(9) 2_575 2_575
O16 W1 O4 93.4(9) . 2_575
O14 W1 O2 159.0(8) . .
O6 W1 O2 97.6(10) . .
O20 W1 O2 93.6(9) . .
O9 W1 O2 65.5(8) 2_575 .
O16 W1 O2 64.6(9) . .
O4 W1 O2 40.6(5) 2_575 .
O15 W2 O10 105.0(13) . .
O15 W2 O16 100.5(11) . .
O10 W2 O16 90.3(9) . .
O15 W2 O12 101.2(10) . 2_575
O10 W2 O12 87.6(8) . 2_575
O16 W2 O12 158.0(10) . 2_575
O15 W2 O13 99.9(9) . 2_575
O10 W2 O13 155.0(12) . 2_575
O16 W2 O13 87.7(7) . 2_575
O12 W2 O13 85.0(9) 2_575 2_575
O15 W2 O3 159.8(9) . 2_575
O10 W2 O3 63.1(11) . 2_575
O16 W2 O3 96.0(9) . 2_575
O12 W2 O3 63.7(8) 2_575 2_575
O13 W2 O3 92.3(7) 2_575 2_575
O15 W2 O2 158.6(9) . .
O10 W2 O2 92.0(12) . .
O16 W2 O2 66.0(9) . .
O12 W2 O2 92.2(8) 2_575 .
O13 W2 O2 64.5(7) 2_575 .
O3 W2 O2 41.3(4) 2_575 .
O19 W3 O20 102.8(10) . .
O19 W3 O17 99.6(9) . .
O20 W3 O17 87.7(7) . .
O19 W3 O7 100.8(9) . .
O20 W3 O7 90.7(9) . .
O17 W3 O7 159.4(10) . .
O19 W3 O8 100.5(12) . .
O20 W3 O8 156.5(13) . .
O17 W3 O8 85.6(8) . .
O7 W3 O8 87.8(8) . .
O19 W3 O1 157.0(7) . .
O20 W3 O1 95.8(9) . .
O17 W3 O1 94.3(8) . .
O7 W3 O1 65.4(8) . .
O8 W3 O1 62.3(10) . .
O19 W3 O4 159.8(7) . 2_575
O20 W3 O4 64.2(8) . 2_575
O17 W3 O4 65.9(7) . 2_575
O7 W3 O4 95.0(8) . 2_575
O8 W3 O4 92.6(11) . 2_575
O1 W3 O4 43.0(4) . 2_575
O18 W4 O11 101.5(11) . .
O18 W4 O12 103.3(9) . .
O11 W4 O12 87.3(8) . .
O18 W4 O17 99.8(10) . .
O11 W4 O17 158.4(11) . .
O12 W4 O17 90.8(9) . .
O18 W4 O6 97.9(10) . .
O11 W4 O6 87.8(8) . .
O12 W4 O6 158.9(11) . .
O17 W4 O6 86.4(6) . .
O18 W4 O3 160.0(8) . .
O11 W4 O3 65.1(8) . .
O12 W4 O3 62.9(8) . .
O17 W4 O3 95.0(9) . .
O6 W4 O3 96.4(9) . .
O18 W4 O4 158.2(8) . 2_575
O11 W4 O4 91.9(9) . 2_575
O12 W4 O4 94.4(8) . 2_575
O17 W4 O4 66.8(8) . 2_575
O6 W4 O4 65.3(9) . 2_575
O3 W4 O4 41.7(4) . 2_575
O22 W5 O5 104.0(12) . .
O22 W5 O7 100.2(9) . .
O5 W5 O7 89.6(8) . .
O22 W5 O10 101.9(12) . .
O5 W5 O10 154.1(15) . .
O7 W5 O10 84.5(9) . .
O22 W5 O11 100.5(9) . 2_575
O5 W5 O11 89.6(10) . 2_575
O7 W5 O11 158.8(10) . 2_575
O10 W5 O11 87.1(7) . 2_575
O22 W5 O1 160.8(7) . .
O5 W5 O1 63.7(10) . .
O7 W5 O1 66.6(8) . .
O10 W5 O1 90.9(12) . .
O11 W5 O1 94.3(9) 2_575 .
O22 W5 O3 156.6(7) . 2_575
O5 W5 O3 94.0(11) . 2_575
O7 W5 O3 94.7(9) . 2_575
O10 W5 O3 61.5(10) . 2_575
O11 W5 O3 64.3(8) 2_575 2_575
O1 W5 O3 42.5(4) . 2_575
O21 W6 O8 102.3(12) . .
O21 W6 O13 101.3(8) . .
O8 W6 O13 88.7(9) . .
O21 W6 O9 99.7(9) . .
O8 W6 O9 157.9(12) . .
O13 W6 O9 88.8(8) . .
O21 W6 O5 102.5(11) . .
O8 W6 O5 88.5(8) . .
O13 W6 O5 156.1(12) . .
O9 W6 O5 84.9(9) . .
O21 W6 O1 159.4(6) . .
O8 W6 O1 64.4(10) . .
O13 W6 O1 94.4(7) . .
O9 W6 O1 93.9(8) . .
O5 W6 O1 63.2(10) . .
O21 W6 O2 159.3(7) . 2_575
O8 W6 O2 93.2(11) . 2_575
O13 W6 O2 65.1(7) . 2_575
O9 W6 O2 66.0(8) . 2_575
O5 W6 O2 91.4(11) . 2_575
O1 W6 O2 41.3(4) . 2_575
O2 Si1 O2 180.000(5) . 2_575
O2 Si1 O3 69.6(9) . 2_575
O2 Si1 O3 110.4(9) 2_575 2_575
O2 Si1 O3 110.4(9) . .
O2 Si1 O3 69.6(9) 2_575 .
O3 Si1 O3 180.0(3) 2_575 .
O2 Si1 O4 111.7(10) . .
O2 Si1 O4 68.3(10) 2_575 .
O3 Si1 O4 70.5(10) 2_575 .
O3 Si1 O4 109.5(10) . .
O2 Si1 O4 68.3(10) . 2_575
O2 Si1 O4 111.7(10) 2_575 2_575
O3 Si1 O4 109.5(10) 2_575 2_575
O3 Si1 O4 70.5(10) . 2_575
O4 Si1 O4 180.000(3) . 2_575
O2 Si1 O1 110.5(10) . .
O2 Si1 O1 69.5(10) 2_575 .
O3 Si1 O1 71.7(10) 2_575 .
O3 Si1 O1 108.3(10) . .
O4 Si1 O1 106.4(9) . .
O4 Si1 O1 73.6(9) 2_575 .
O2 Si1 O1 69.5(10) . 2_575
O2 Si1 O1 110.5(10) 2_575 2_575
O3 Si1 O1 108.3(10) 2_575 2_575
O3 Si1 O1 71.7(10) . 2_575
O4 Si1 O1 73.6(9) . 2_575
O4 Si1 O1 106.4(9) 2_575 2_575
O1 Si1 O1 180.000(2) . 2_575
Si1 O1 O2 54.4(6) . 2_575
Si1 O1 O3 53.8(6) . 2_575
O2 O1 O3 89.6(10) 2_575 2_575
Si1 O1 O4 52.8(5) . 2_575
O2 O1 O4 89.2(9) 2_575 2_575
O3 O1 O4 86.6(9) 2_575 2_575
Si1 O1 W6 124.7(10) . .
O2 O1 W6 70.3(9) 2_575 .
O3 O1 W6 133.9(12) 2_575 .
O4 O1 W6 132.1(12) 2_575 .
Si1 O1 W5 123.7(11) . .
O2 O1 W5 131.4(12) 2_575 .
O3 O1 W5 69.9(9) 2_575 .
O4 O1 W5 130.6(12) 2_575 .
W6 O1 W5 92.5(4) . .
Si1 O1 W3 122.4(10) . .
O2 O1 W3 132.4(13) 2_575 .
O3 O1 W3 128.8(12) 2_575 .
O4 O1 W3 69.6(9) 2_575 .
W6 O1 W3 92.6(5) . .
W5 O1 W3 91.9(5) . .
Si1 O2 O4 56.3(6) . 2_575
Si1 O2 O3 55.6(6) . 2_575
O4 O2 O3 93.0(10) 2_575 2_575
Si1 O2 O1 56.1(6) . 2_575
O4 O2 O1 91.0(10) 2_575 2_575
O3 O2 O1 91.4(10) 2_575 2_575
Si1 O2 W2 124.3(10) . .
O4 O2 W2 130.5(14) 2_575 .
O3 O2 W2 68.7(9) 2_575 .
O1 O2 W2 133.0(14) 2_575 .
Si1 O2 W6 124.5(12) . 2_575
O4 O2 W6 130.9(12) 2_575 2_575
O3 O2 W6 129.8(14) 2_575 2_575
O1 O2 W6 68.4(10) 2_575 2_575
W2 O2 W6 91.8(5) . 2_575
Si1 O2 W1 123.6(12) . .
O4 O2 W1 67.2(10) 2_575 .
O3 O2 W1 132.8(14) 2_575 .
O1 O2 W1 129.3(12) 2_575 .
W2 O2 W1 91.6(5) . .
W6 O2 W1 91.5(4) 2_575 .
Si1 O3 O2 54.7(6) . 2_575
Si1 O3 O4 54.7(6) . 2_575
O2 O3 O4 91.9(10) 2_575 2_575
Si1 O3 O1 54.5(6) . 2_575
O2 O3 O1 90.4(10) 2_575 2_575
O4 O3 O1 87.3(9) 2_575 2_575
Si1 O3 W2 124.7(10) . 2_575
O2 O3 W2 70.0(9) 2_575 2_575
O4 O3 W2 136.4(13) 2_575 2_575
O1 O3 W2 130.4(13) 2_575 2_575
Si1 O3 W4 124.2(12) . .
O2 O3 W4 131.5(14) 2_575 .
O4 O3 W4 69.5(10) 2_575 .
O1 O3 W4 130.7(11) 2_575 .
W2 O3 W4 92.8(5) 2_575 .
Si1 O3 W5 122.1(11) . 2_575
O2 O3 W5 132.3(14) 2_575 2_575
O4 O3 W5 126.6(12) 2_575 2_575
O1 O3 W5 67.6(9) 2_575 2_575
W2 O3 W5 92.1(5) 2_575 2_575
W4 O3 W5 91.7(4) . 2_575
Si1 O4 O2 55.4(6) . 2_575
Si1 O4 O3 54.7(6) . 2_575
O2 O4 O3 91.9(11) 2_575 2_575
Si1 O4 O1 53.6(6) . 2_575
O2 O4 O1 90.0(9) 2_575 2_575
O3 O4 O1 87.3(9) 2_575 2_575
Si1 O4 W1 127.5(11) . 2_575
O2 O4 W1 72.2(10) 2_575 2_575
O3 O4 W1 134.3(12) 2_575 2_575
O1 O4 W1 133.6(12) 2_575 2_575
Si1 O4 W4 123.4(11) . 2_575
O2 O4 W4 135.6(13) 2_575 2_575
O3 O4 W4 68.7(9) 2_575 2_575
O1 O4 W4 126.5(12) 2_575 2_575
W1 O4 W4 92.8(4) 2_575 2_575
Si1 O4 W3 121.0(10) . 2_575
O2 O4 W3 130.4(13) 2_575 2_575
O3 O4 W3 128.2(12) 2_575 2_575
O1 O4 W3 67.4(9) 2_575 2_575
W1 O4 W3 91.7(5) 2_575 2_575
W4 O4 W3 90.4(5) 2_575 2_575
W5 O5 W6 139.8(15) . .
W1 O6 W4 134.4(16) . .
W5 O7 W3 135.8(12) . .
W6 O8 W3 140.0(17) . .
W6 O9 W1 136.6(11) . 2_575
W2 O10 W5 142.4(17) . .
W4 O11 W5 138.5(12) . 2_575
W2 O12 W4 139.9(13) 2_575 .
W6 O13 W2 137.9(11) . 2_575
W2 O16 W1 137.5(14) . .
W3 O17 W4 136.6(11) . .
W3 O20 W1 137.4(12) . .
N1 Cu1 N6 118.4(8) . .
N1 Cu1 N4 113.0(8) . 2_564
N6 Cu1 N4 128.4(8) . 2_564
N5 Cu2 N2 146.8(10) . .
N5 Cu2 N3 110.4(10) . .
N2 Cu2 N3 102.2(8) . .
C4 N1 C1 113(2) . .
C4 N1 Cu1 119.7(17) . .
C1 N1 Cu1 126.6(17) . .
C2 C1 N1 129(2) . .
C1 C2 N2 119(3) . .
N2 C3 C4 120(2) . .
N1 C4 C3 121(2) . .
C3 N2 C2 118(2) . .
C3 N2 Cu2 121(2) . .
C2 N2 Cu2 118.9(19) . .
C8 N3 C5 114.3(17) . .
C8 N3 Cu2 118.9(15) . .
C5 N3 Cu2 126.7(15) . .
C6 C5 N3 123.4(19) . .
C5 C6 N4 122.5(19) . .
N4 C7 C8 123.9(18) . .
N3 C8 C7 119.7(17) . .
C7 N4 C6 115.7(18) . .
C7 N4 Cu1 120.0(15) . 2_564
C6 N4 Cu1 124.0(13) . 2_564
C10 N5 C9 118.5(18) . .
C10 N5 Cu2 122(2) . .
C9 N5 Cu2 119(2) . .
N5 C9 C10 115(3) . 2_454
N5 C10 C9 126(3) . 2_454
C12 N6 C11 114.6(18) 2_665 .
C12 N6 Cu1 123.7(15) 2_665 .
C11 N6 Cu1 121.6(15) . .
C12 C11 N6 118(2) . .
C11 C12 N6 127(2) . 2_665
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
W1 O14 1.675(16) .
W1 O6 1.878(18) .
W1 O20 1.903(16) .
W1 O9 1.907(19) 2_575
W1 O16 1.920(17) .
W1 O4 2.386(17) 2_575
W1 O2 2.463(19) .
W2 O15 1.667(18) .
W2 O10 1.835(18) .
W2 O16 1.85(2) .
W2 O12 1.86(2) 2_575
W2 O13 1.919(18) 2_575
W2 O3 2.419(16) 2_575
W2 O2 2.440(17) .
W3 O19 1.689(17) .
W3 O20 1.861(19) .
W3 O17 1.886(17) .
W3 O7 1.91(2) .
W3 O8 1.934(18) .
W3 O1 2.461(18) .
W3 O4 2.498(18) 2_575
W4 O18 1.674(15) .
W4 O11 1.877(19) .
W4 O12 1.88(2) .
W4 O17 1.895(14) .
W4 O6 1.93(2) .
W4 O3 2.439(19) .
W4 O4 2.452(18) 2_575
W5 O22 1.648(14) .
W5 O5 1.84(2) .
W5 O7 1.88(2) .
W5 O10 1.88(2) .
W5 O11 1.89(2) 2_575
W5 O1 2.428(18) .
W5 O3 2.468(19) 2_575
W6 O21 1.697(13) .
W6 O8 1.82(2) .
W6 O13 1.845(18) .
W6 O9 1.88(2) .
W6 O5 1.894(19) .
W6 O1 2.423(17) .
W6 O2 2.454(19) 2_575
Si1 O2 1.492(8) .
Si1 O2 1.492(8) 2_575
Si1 O3 1.509(9) 2_575
Si1 O3 1.509(9) .
Si1 O4 1.509(9) .
Si1 O4 1.509(9) 2_575
Si1 O1 1.523(9) .
Si1 O1 1.523(9) 2_575
O1 O2 1.72(2) 2_575
O1 O3 1.78(2) 2_575
O1 O4 1.82(2) 2_575
O2 O4 1.68(2) 2_575
O2 O3 1.71(2) 2_575
O2 O1 1.72(2) 2_575
O2 W6 2.454(19) 2_575
O3 O2 1.71(2) 2_575
O3 O4 1.74(2) 2_575
O3 O1 1.78(2) 2_575
O3 W2 2.419(16) 2_575
O3 W5 2.468(19) 2_575
O4 O2 1.68(2) 2_575
O4 O3 1.74(2) 2_575
O4 O1 1.82(2) 2_575
O4 W1 2.386(17) 2_575
O4 W4 2.452(18) 2_575
O4 W3 2.498(18) 2_575
O9 W1 1.907(19) 2_575
O11 W5 1.89(2) 2_575
O12 W2 1.86(2) 2_575
O13 W2 1.919(18) 2_575
Cu1 N1 1.941(17) .
Cu1 N6 1.943(19) .
Cu1 N4 1.967(18) 2_564
Cu2 N5 1.87(2) .
Cu2 N2 1.934(17) .
Cu2 N3 2.034(19) .
N1 C4 1.27(3) .
N1 C1 1.35(3) .
C1 C2 1.29(4) .
C2 N2 1.36(3) .
C3 N2 1.24(4) .
C3 C4 1.52(4) .
N3 C8 1.36(3) .
N3 C5 1.43(3) .
C5 C6 1.27(3) .
C6 N4 1.36(3) .
C7 N4 1.34(3) .
C7 C8 1.37(3) .
N4 Cu1 1.967(18) 2_564
N5 C10 1.343(10) .
N5 C9 1.344(10) .
C9 C10 1.52(4) 2_454
C10 C9 1.52(4) 2_454
N6 C12 1.33(3) 2_665
N6 C11 1.43(3) .
C11 C12 1.28(3) .
C12 N6 1.33(3) 2_665
